d Nephila clavipes silk produced naturally and through controlled silking. e Rat-
tail collagen Type I extruded fibers tested after stretching from 0% to 50%.
Biomaterials 24 (2003) 401–416
Silk-based biomaterials Gregory H. Altman, Frank Diaz, Caroline Jakuba, Tara Calabro, Rebecca L. Horan, Jingsong Chen, Helen Lu, John Richmond, David L. Kaplan* Department of Chemical and Biological Engineering, Bioengineering Center, Tufts University, 4 Colby Street, Medford, MA 02155, USA Received 17 April 2002; accepted 19 June 2002
Abstract Silk from the silkworm, Bombyx mori, has been used as biomedical suture material for centuries. The unique mechanical properties of these ﬁbers provided important clinical repair options for many applications. During the past 20 years, some biocompatibility problems have been reported for silkworm silk; however, contamination from residual sericin (glue-like proteins) was the likely cause. More recent studies with well-deﬁned silkworm silk ﬁbers and ﬁlms suggest that the core silk ﬁbroin ﬁbers exhibit comparable biocompatibility in vitro and in vivo with other commonly used biomaterials such as polylactic acid and collagen. Furthermore, the unique mechanical properties of the silk ﬁbers, the diversity of side chain chemistries for ‘decoration’ with growth and adhesion factors, and the ability to genetically tailor the protein provide additional rationale for the exploration of this family of ﬁbrous proteins for biomaterial applications. For example, in designing scaffolds for tissue engineering these properties are particularly relevant and recent results with bone and ligament formation in vitro support the potential role for this biomaterial in future applications. To date, studies with silks to address biomaterial and matrix scaffold needs have focused on silkworm silk. With the diversity of silk-like ﬁbrous proteins from spiders and insects, a range of native or bioengineered variants can be expected for application to a diverse set of clinical needs. r 2002 Elsevier Science Ltd. All rights reserved. Keywords: Silk; Sericin; Fibroin; Foreign body response; Suture; Tissue engineering; Biomaterial; Scaffold
1. Background Silks are generally deﬁned as protein polymers that are spun into ﬁbers by some lepidoptera larvae such as silkworms, spiders, scorpions, mites and ﬂies [1–3]. Silk proteins are usually produced within specialized glands after biosynthesis in epithelial cells, followed by secretion into the lumen of these glands where the proteins are stored prior to spinning into ﬁbers. Silks differ widely in composition, structure and properties depending on the speciﬁc source. The most extensively characterized silks are from the domesticated silkworm, Bombyx mori, and from spiders (Nephila clavipes and Araneus diadematus). Many of the more evolutionarily advanced spiders synthesize different types of silks. Each of these different silks has a different amino acid composition and exhibits mechanical properties tailored *Corresponding author. Tel.: +1-617-627-3251; fax: +1-617-6273231. E-mail address: [email protected]
to their speciﬁc functions: reproduction as cocoon capsular structures, lines for prey capture, lifeline support (dragline), web construction and adhesion. Fibrous proteins, such as silks and collagens, are characterized by a highly repetitive primary sequence that leads to signiﬁcant homogeneity in secondary structure, i.e., triple helices in the case of collagens and b-sheets in the case of many of the silks. These types of proteins usually exhibit important mechanical properties, in contrast to the catalytic and molecular recognition functions of globular proteins. Because of these impressive mechanical properties, this family of proteins provides an important set of material options in the ﬁelds of controlled release, biomaterials and scaffolds for tissue engineering. The relative environmental stability of these families of proteins, in comparison to globular proteins, in combination with their biocompatibility, unique mechanical properties, and options for genetic control to tailor sequence provides an important basis to exploit these natural proteins for biomedical applications.
0142-9612/02/$ - see front matter r 2002 Elsevier Science Ltd. All rights reserved. PII: S 0 1 4 2 - 9 6 1 2 ( 0 2 ) 0 0 3 5 3 - 8
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
1.1. Silkworm silk Silkworm silk has been used commercially as biomedical sutures for decades, and in textile production for centuries. The silk from the cocoon of B. mori contains at least two major ﬁbroin proteins, light and heavy chains, 25 and 325 kDa, respectively. These core ﬁbers are encased in a sericin coat, a family of glue-like proteins that holds two ﬁbroin ﬁbers together to form the composite ﬁbers of the cocoon case to protect the growing worm. This structural arrangement contrasts with spider silks where these glue-like proteins are generally absent. Silkworm cocoon silk production, known as sericulture, produces high yields since the larvae can be maintained in high densities. The core sequence repeats in the ﬁbroin heavy chain from B. mori include alanine–glycine repeats with serine or tyrosine. 1.2. Spider silks Spider silks have not been commercialized for biomedical applications primarily due to the predatory nature of spiders and the relatively low levels of production of these silks when compared to silkworm cocoon silk. The molecular weights of spider silk proteins vary depending on source but can range from 70 to 700 kDa depending on the method of analysis. The dragline silk from N. clavipes is characterized by polyalanine and glycine–glycine-X regions, where X is often tyrosine, glutamine or leucine. Genetic engineering is being actively explored to construct, clone and express native and synthetic genes encoding recombinant spider silk proteins to overcome limits to use of the native organisms. This strategy has provided new opportunities in fundamental studies of spider silk genetics, silk protein structure and function, and materials processing [2,4–6]. In general, interest in spider silk has increased in recent years due to the differences in mechanical properties when compared to silkworm silk and the presence of the multi-gene family encoding this group of silks as a basis for the study of protein structurefunction relationships [4,6–11]. During the past 10 years a great deal of progress has been made in understanding silk genetic and protein structures. Cloning and expression of native and synthetic silks has been achieved in a variety of host systems. The sequences of cDNAs and genomic clones encoding spider silks illustrate the highly repetitive structures [4,6,8–11], which can be readily exploited to construct genetically engineered spider silk-like proteins using synthetic oligonucleotide versions of the consensus repeats or variants of these repeats. This highly repetitive sequence was also recently fully described for the ﬁbroin heavy chain from the silkworm, B. mori . The unique organization of the family of silk genes in more advanced spiders provides a fertile area for the
exploration of structure-function relationships in protein design. For example, the dragline spider silk from the golden orb weaver N. clavipes displays impressive toughness, and a balance of stiffness, strength and extensibility reﬂecting the native function of the silk orb web construction [7,13,14]. Transgenic expression of spider silks in plants (tobacco and potato) and mammalian epithelial cells has been reported [15,16] and may point the way toward more substantive production of these proteins in the future. Furthermore, since native and genetically engineered versions of the silks tend to self-assemble into microﬁbrils, causing precipitation and leading to loss of protein during puriﬁcation [3,17], alternative methods to maintain solubility of the recombinant versions of these proteins have been explored. For example, tweaking the native or consensus sequences of spider silks to include encoded ‘triggers’ to regulate molecular-level assembly of the proteins has been demonstrated [17–21]. Chemical redox triggers, or a kinase recognition site for biochemical phosphorylation, ﬂanking the b-sheet forming regions of the proteins have been demonstrated. These modiﬁcations encoded in the synthetic gene designs enabled improved control over solubility of the genetically engineered silk protein. 1.3. Properties of silk The enhanced environmental stability of silk ﬁbers in comparison to globular proteins is due to the extensive hydrogen bonding, the hydrophobic nature of much of the protein, and the signiﬁcant crystallinity. Silks are insoluble in most solvents, including water, dilute acid and alkali. Detailed structural analysis of spider dragline silk proteins has yielded information on the organization and orientation of the numerous but very small b-sheet crystals in the ﬁbers, and a high level of organization of the protein even in the less crystalline domains . Liquid crystalline phases and conformational polymorphism have been implicated in the biological processing of these proteins to contribute to the architectural features within the ﬁbers [22–24]. These nanoscale features, factoring in the small, orientated and numerous b-sheet crystals, a fuzzy interphase between these crystals and the less crystalline domains, and the shear alignment of the chains, provides a basis for the origin of the novel mechanical properties exhibited by silk ﬁbers. A comparison of mechanical properties (Table 1) suggests that they provide a remarkable combination of strength and toughness. The distinguishing features of the spider silks are the very high strength in combination with excellent elasticity in comparison with these other biomaterials. In addition, these ﬁbers display resistance to failure in compression that distinguishes them from other high performance ﬁbers, such as Kevlar .
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
Table 1 Comparison of mechanical properties of common silks (silkworm and spider dragline) to several types of biomaterial ﬁbers and tissues commonly used today Material a
B. mori silk (w/ sericin) B. mori silk (w/o sericin)b B. mori silkc Spider silkd Collagene Collagen X-linkedf PLAg Tendon (comprised of mainly collagen) Bone Kevlar (49 ﬁber) Synthetic Rubber
% Strain at break
500 610–690 740 875–972 0.9–7.4 47–72 28–50 150 160 3600 50
5–12 15–17 10 11–13 0.0018–0.046 0.4–0.8 1.2–3.0 1.5 20 130 0.001
19 4–16 20 17–18 24–68 12–16 2–6 12 3 2.7 850
Perez-Rigueiro et al.  Perez-Rigueiro et al.  Cunniff et al.  Cunniff et al.  Pins et al.  Pins et al.  Engelberg and Kohn  Gosline et al.  Gosline et al.  Gosline et al.  Gosline et al. 
Bombyx mori silkworm silk—determined from bave (multithread ﬁbers naturally produced from the silk worm coated in sericin). Bombyx mori silkworm silk—determined from single brins (individual ﬁbroin ﬁlaments following extraction of sericin). c Bombyx mori silkworm silk—average calculated from data in Ref. . d Nephila clavipes silk produced naturally and through controlled silking. e Rat-tail collagen Type I extruded ﬁbers tested after stretching from 0% to 50%. f Rat-tail collagen dehydrothermally cross-linked and tested after stretching from 0% to 50%. g Polylactic acid with molecular weights ranging from 50,000 to 300,000. b
2. Utility in biomedical applications B. mori silkworm silk ﬁbers have been the primary silk-like material used in biomedical applications particularly as sutures. During decades of use, silk ﬁbers have proven to be effective in many clinical applications. At the same time, some biological responses to the protein have raised questions about biocompatibility. One of the major difﬁculties in assessing the biological responses reported to these silk ﬁbers is the absence of detailed characterization of the ﬁbers used including, extent of extraction of the sericin, the chemical nature of wax-like coatings sometimes used, and many related processing factors. This variability in source material has resulted in confusion in the literature and in clinical settings concerning the beneﬁts or potential concerns with this class of ﬁbrous protein. For example, of greatest importance is that based on many studies it is clear that the sericin glue-like proteins are the major cause of adverse problems with biocompatibility and hypersensitivity to silk (Table 2). If sericin is removed, the biological responses to the core ﬁbroin ﬁbers appear to be comparable to most other commonly used biomaterials (Table 3). An additional major misconception revolves around silk’s classiﬁcation as non-degradable. There is clear evidence in the literature that silk, as a protein, is susceptible to proteolytic degradation in vivo and over longer time periods in vivo will slowly be absorbed.
3. In vivo biocompatibility of virgin silk Despite centuries of use as sutures , silk matrices are now being rediscovered and reconsidered as
potentially useful biomaterials for a range of applications in clinical repairs and in vitro as scaffolds for tissue engineering ; some beneﬁts and concerns of silk are detailed in Table 4. Silk has been used most extensively as sutures for wound ligation and became the most common natural suture surpassing collagen (CatgutTM or Chromic CatgutTM, cross-linked collagen) used in the biomedical industry over the past 100 years . During the past 20 years, a variety of degradable synthetic materials including polyglycolic acid (PGA)(DexonTM), co-polymers of PGA (polyglyconate)(MaxonTM or gylcolide and trimethylene carbonate), and co-polymers of PGA and polylactic acid (VicrylTM or polyglactin 910, a co-polymer of 90% glycolide and 10% l-lactide), polydioxanone (PDS), and non-degradable synthetics including braided polyester (EthibondTM or MersileneTM), nylon (EthilonTM), Teﬂon coated polyester (TevdekTM) and polypropylene (ProleneTM or SurgileneTM) have dominated the suture market. In general, sutures should be strong, handle easily, and form secure knots . Sutures require the following characteristics for general surgical applications : 1. Tensile strength—to match the clinical repair. 2. Knot strength—the amount of force required to cause a knot to slip. 3. Elasticity—the ability to conform to the current stage of wound repair. 4. Memory—change in stiffness over time; the better the suture, the less memory. 5. Degradability—ability to be metabolized by the host once its repair function has been completed. 6. Tissue Reactivity—non-irritant.
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
404 Table 2 Biological responses to virgin silk ﬁbers Type of silka
In vivo or in vitro model/tissue site
Mucosal edema was greatest around silk and chromic collagen compared to PGA Chronic inﬂammation including granulosous and ﬁbrosis
Morrow et al. 
Rabbit/median or sciatic nerve ligation Human/ocular cataract surgery
Nebel et al. 
Black braided Virgin
? Virgin Virgin
(a) Acute and chronic inﬂammation initially including conjunctival and episcleral hyperemia progressing to chemosis and nodular episcleritis, peripheral corneal ulceration and wound necrosis (b) Sensitization to virgin silk during bilateral cataract surgery following the use of virgin silk on the ﬁrst eye No comparable suture reactions IgE obtain from sera isolated from 8 of 9 patients with allergy to silk bound speciﬁcally to sericin and was negative towards ﬁbroin (a) Acute and chronic inﬂammation (b) However, the response was not signiﬁcantly different from VicrylTM, Chromic Catgut, TevdekTM and polypropylene Severe delayed chronic inﬂammatory reaction to suture Delayed hypersensitivity to virgin silk resulting in asthma (a) 90% of patient population developed an allergic reaction to silk extract (sericin); none of the control group was allergic (b) IgE from 41% of the patient population sera bound speciﬁcally to sericin in in vitro testing (a) Type I allergy response to black braided silk
Human/ocular cataract surgery In vitro immunoblot of IgE and IgG isolated from sera of 9 persons allergic to silk Rabbit/tracheal anastomosis
Three human pediatric patients/ neurosurgery Children o15 yr old/skin tests 41 humans with asthma and a clinical history of silk allergy; 4 control patients with no allergy to silk/sera and skin tests were used.
Single case in a human/trachea and throat region
Soong and Kenyon 
Soong and Kenyon  Dewair et al. 
Peleg et al. 
Rossitch et al.  Wen et al.  Zaoming et al. 
Kurosaki et al. 
(b) Patient sensitized to silk 7 years prior in an independent surgical procedure a ?=Type of silk used was not speciﬁed, e.g., virgin silk or black braided; Virgin=virgin silk containing sericin; Black braided=black braided extracted silk ﬁbroin (e.g., no sericin) coated in waxes or silicone.
7. Free from infection—related to the material’s geometry, e.g., multiﬁlament vs. monoﬁlament. Processing methods for virgin silk (ﬁbroin containing sericin gum) were developed in industry to extract sericin from the inner silk ﬁbroin ﬁbers. As sutures, the silk ﬁbroin ﬁbers are usually coated with waxes or silicone to enhance material properties and reduce fraying; these sutures are commonly referred to as black braided silk (e.g., Perma-HandTM). The transition from virgin silk to black braided sutures occurred in the late 1970s and early 1980s; however, virgin silk is still commercially available today. Virgin silk, like most proteins, is a potential allergen [28,29] causing a Type I allergic response in some cases . Delayed allergic responses to silk (an average of 10 months after initial exposure) induced some patient complications including asthma and speciﬁc upregulation in IgE levels [29,31]. Wen et al.  showed the extracted sericin was responsible for sensitization (the development of a T-cell mediated allergic response) by
skin testing of 64 children with asthma. Further biochemical analysis by Dewair et al.  and Zaoming et al.  concluded that upregulated IgEs were produced in response to the sericin, clarifying the role of these ﬁbroin contaminants as the main allergenic agent in silk and not the core ﬁbroin ﬁbers. Fibroin degradation products could also potentially be involved in adverse biological responses. For example, one case was reported where ﬁbroin (black braided silk) may have induced a Type I allergic reaction . However, the authors clariﬁed later that there were no cases in the literature that implicated black braided silk as inducer of IgE hypersensitivity reactions. In addition, in the preparation of this review no references were found in the literature that implicated black braided silk in inducing hypersensitivity and allergic reactions. Kurosaki et al.  concluded that the hypersensitivity in their single case may have been the result of patient sensitization to silk from a prior surgical procedure 7 years earlier. The type of silk used in this earlier exposure was unknown (e.g., virgin vs. black braided).
Rat/ Abdominal incision
Minimal Minimal Minimal Moderate
Yes; o60 days No No Yes; o60 days Yes; >60 days
8.2% (7.3–10.6) 8.7% (7.1–9.9) 9.48% (8.3–15) 11.25% (9.5–12.7) 14.2% (10.9–22.3) 15.8% (12.1–19.1) Mild (1) Mild (1) Mild (1) Moderate (2) Moderate (2) Moderate (2) Moderate (2) Moderate (2) Moderate (2)
o60 days o60 days >60 days
o60 days o60 days o60 days >60 days
Foreign body response
— Yes; Yes; Yes; Yes; No No No No Yes; Yes; Yes; No No
Mono Multi Multi Multi
— Multi Multi Multi Multi Mono Mono Mono Mono Multi Multi Multi Mono Multi
Bucknall et al. 
Setzen et al. 
Foschi et al. 
Absorbable is deﬁned as the loss of tensile strength within 60 days in vivo, but does not reﬂect the persistence of a foreign body response (FBR) for greater than 60 days. Monoﬁlament sutures contain a single ﬁber and multiﬁlament sutures contain multiple ﬁbers increasing material surface area in vivo and the potential risk of infection (i.e., more places for contamination to hide in multiﬁlament sutures). c FRB was characterized by the percent growth of neovessels (angiogenesis) around the suture 7 days post-implantation. d FBR was characterized on a 3 level scale 30 days post-implantation: Mild (1) included the presence of histiocytes and foreign-body giant cells, Moderate (2) indicates histiocytes and foreign-body giant cells, and cluster of lymphocytes and a few plasmacytes, and Extensive (3) includes histiocytes, foreign-body giant cells, and diffuse, scattered lymphocytes and plasmacytes. e FBR was characterized histologically 10 days in vivo; however, the authors do not provide a deﬁnition of ‘minimal’ or ‘moderate’ inﬂammation and provide no means by which they systematically characterize the response histologically.
Rat/ Abdominal cavity
Surgical control VicrylTM (polyglactin 910) CatgutTM (Collagen) Polyglycolic acid salt (PGA) Silk (assumed black braided) Titanium (metal clip) Extruded TeﬂonTM ProleneTM (polypropylene) SurgileneTM (polypropylene) PDSTM (polydioxanone) VicrylTM Silk (black braided) Nylon EthibondTM (braided polyester) MersilineTM (braided polyester) TevdekTM (Teﬂon coated polyester) Chromic CatgutTM (cross linked collagen) Nylon Nylon PGA Silk (black braided)
Suture trade name/material
Table 3 Common sutures that elicit a foreign body response following implantation in vivo
G.H. Altman et al. / Biomaterials 24 (2003) 401–416 405
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
Table 4 Beneﬁts and concerns with the use of silks for biomedical applications Benefits Novel mechanical properties of some silks that are superior to any other natural ﬁber and rival many high performance ﬁbers Natural ﬁber with a long standing history of use in clinical applications The ability to process silks in aqueous solutions for subsequent formation of ﬁlms and other material formats, with relatively simple insolubilization via exposure to alcohols and other environmental factors Easily chemically modiﬁed with surface decorations, such as adhesion sites or cytokines, due to the availability of amine and acid side chains on some of the amino acids Genetically tailorable composition and sequence to moderate speciﬁc features, such as molecular weight, crystallinity, solubility Slow rates of degradation in vitro and in vivo, this is particularly useful in biodegradable scaffolds in which slow tissue ingrowth is desirable No known risk of bioburden Concerns Adequate removal of contaminating sericin from silkworm silk to avoid biocompatibility problems Slow degradation of crystalline (b-sheet) regions Aborted proteolytic attack by macrophages and giant cells leading to encapsulation and the formation of a granuloma Potential sensitization to silk ﬁbroin resulting in an allergic response upon exposure to the biomaterial
In other cases where the type of silk suture was unknown , silk induced a delayed allergic reaction that necessitated the removal of the suture. The authors did not distinguish between the use of virgin silk containing sericin versus black braided silk. However, based on the time frame of the surgical procedures (1970s) and the severity of the reaction, sericin can be considered as the most likely cause of the response. Soong and Kenyon  detailed 12 patients from 1980 to 1983 that reported severe reactions to virgin silk sutures following cataract surgery. No comparable reactions were noted when black-braided silk sutures were used. Further, they provided evidence of patient sensitization to virgin silk in bilateral surgical procedures; an allergic reaction developed against virgin silk following its use in the ﬁrst eye procedure. The use of virgin silk during the 1960s to the early 1980s negatively impacted the general acceptance of this biomaterial from the surgical practitioner perspective [35–37]. For example, Morrow et al.  observed silk and collagen (catgut) to be moderately more reactive than polyglycolic acid (PGA) in the genitourinary tract following 3 weeks of implantation in vivo, although again the type of silk used in the study was not identiﬁed. Nebel et al.  observed cellular inﬁltration, granulosous and ﬁbrosis for silk sutures that persisted for more than 4 weeks compared to autologous collagen sutures used for peripheral nerve ligation in the rabbit. Again the speciﬁc type of silk was not described. Of note in the study was that inﬂammation was comparable to chromic collagen sutures. Peleg et al.  drew a similar conclusion regarding the inﬂammatory potential of silk used in tracheal anastomosis in the rabbit without identifying the type of silk used. Of interest was a similar acute and chronic inﬂammatory response to VicrylTM and TeﬂonTM coated polyester sutures in the study.
4. Foreign body response to silk All biomaterials derived from a non-autologous source will elicit some level of foreign body response (FBR) following implantation in vivo. Absorbable and non-degradable biomaterials generally do not induce a T-cell mediated hypersensitivity immune response (as was observed with sericin) . However, while rare, sensitization to ﬁbroin due to pre-exposure or a failed phagocytic response can result in the formation of a granuloma years after the implantation of black braided silk . Some common materials that have been shown to induce a FBR are detailed in Table 3. Biomaterial characteristics, including implantation site, size, geometry , and surface topography can inﬂuence the level of the foreign body response . This response can be predicted in part based on the surface to volume ratio of the biomaterial . This relationship is frequently not addressed in the relative comparison between different suture types in vivo. Several studies have shown black braided silk to elicit a greater FBR when compared to other commonly used sutures [43–45]. However, a single ﬁber of native silk is composed of several individual ﬁbroin ﬁlaments and a single black braided suture comprises several extracted silk ﬁbers. No studies have attempted to normalize the FBR to the suture surface area, rather equating sutures based on their ﬁnal diameter. Thus studies that report silk as inducing a heightened FBR may not be reﬂective of the inﬂammatory potential of the silk but rather a manifestation of the overall suture structure and geometry. Silk sutures induced angiogenesis, a limiting step in mounting a foreign body response, in the rat’s mesenteric window 7 days post-implantation to an lesser extent as titanium and to a greater extent than collagen, polyglactin, and PGA; however the differences
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
were not statistically signiﬁcant ðp > 0:05Þ (Table 3) . The type of silk suture (virgin versus black braided) was not described but it is assumed to be black braided based on the year of study. A curiosity about the study was the choice to close all the wounds of all study groups with silk suture, potentially sensitizing the animals to the silk suture under investigation. Bucknall et al.  examined four sutures in abdominal wound closure in a rat model 10, 30, and 70 days postimplantation. Histological examination revealed silk elicited a ‘moderate’ zone of inﬂammation compared to a ‘minimal response’ induced by multi- and monoﬁlament nylon and multiﬁlament PGA (Table 3). No histological criteria or ranking system was provided. However, the authors noted that even monoﬁlament nylon, thought to be the most biocompatible of the materials evaluated, induced ﬁbrous encapsulation 10 days post-implantation. Of interest was the ﬁnding that PGA, despite a 92% decrease in tensile strength 30 days post-implantation continued to elicit a FBR over 70 days in vivo, the ﬁnal time point of the study. Setzen et al.  in a comprehensive blind study, statistically analyzed tissue responses to 11 types of sutures subcutaneously implanted in the rabbit (Table 3). Responses were based on the number of giant cells present in the ﬁbrous capsule and within the individual ﬁlaments of the sutures, and the thickness of the ﬁbrous capsule surrounding the suture. Evaluations were performed 30, 60 and 120 days post-implantation. The inﬂammatory response surrounding the encapsulation was graded on a scale of 1–3 based on the type of cells and the number of vessels found. Silk elicited an equivalent response to absorbable sutures and multiﬁlament non-absorbable sutures when evaluating the number of foreign body cells surrounding each suture 30 days post-implantation. Non-degradable EthibondTM (braided polyester) and TevdekTM(Teﬂon coated polyester) induced a signiﬁcantly greater accumulation of cells at the wound site compared to the group of sutures under investigation. However, when assessing the thickness of the ﬁbrous capsule, black braided silk as well as EthibondTM induced the formation of signiﬁcantly thicker capsules compared to the mean response of the group. Histological analysis 30 days after implantation showed the tissue response to the silk was equivalent to VicrylTM and PDSTM (two common synthetic absorbables), nylon (monoﬁlament), and EthibondTM, MersileneTM and TevdekTM (three common multiﬁlament non-degradables), and less than cross-linked collagen (Chromic CatgutTM). The foreign body response to VicrylTM lasted in excess of 120 days in vivo, long after the loss of tensile integrity. In conclusion, Setzen et al.  conﬁrmed that the inﬂammatory response induced by silk was no greater than that in response to common absorbable sutures 30 days post-implantation in a subcutaneous rabbit in vivo
model (Table 3). Furthermore, they found a signiﬁcantly higher response to multiﬁlament sutures than monoﬁlament, conﬁrming the inﬂuence of higher surface area to volume ratio as indicative of induction of a greater inﬂammatory response. As a suture, silk is still popular in ocular, neural and cardiovascular surgery, but has also been used in a variety of other tissues in the body. Silk’s knot strength, handling characteristics and ability to lay low to the tissue surface make it a popular suture in cardiovascular applications where bland tissue reactions are desirable for the coherence of the sutured structures . However, black braided silk is thrombotic following implantation within ateriovessels [46,47]. Using a rat model, Dahike et al.  showed black braided silk binds ﬁbrin and platelets within 3 days in vivo following implantation into arteriovessels. Within 7 days, silk was encapsulated by a dense thrombus consisting of platelets and lymphocytes, erythrocytes, and granulocytes. From 14 to 28 days, the gradual decline of the thrombus and the development of a new endothelium layer was observed. By 28 days in vivo, silk was completely endothelialized, indicating the presence of regenerated endothelial tissue. While silk was initially thrombotic (e.g, 3 and 7 days post-implantation) when compared to ProleneTM, EthilonTM, VicrylTM and MersileneTM, by 28 days in vivo, silk was less so when compared to both EthilonTM and VicrylTM. At 56 days post-implantation only traces of thrombogenicity were detected with black braided silk by the presence of loosely bound platelets to the neoendothelium. The ability of black braided silk to induce thrombosis immediately following implantation in blood ﬂow may be due to the surface properties and ability to bind proteins in the clotting cascade such as ﬁbrin. Altering the surface properties of extracted ﬁbroin silk (i.e., eliminating the wax coating) signiﬁcantly diminished the initially high thrombotic response to silk . Sakabe et al.  coated polyester suture with solubilized ﬁbroin and demonstrated that the reconstituted ﬁbroin protein did not induce signiﬁcant thrombogenicity in vivo. In vitro studies performed by Santin et al.  conﬁrmed the ability of silk ﬁbroin ﬁlms (extracted sericin-free ﬁbroin dissolved in LiBr salt, dialyzed in dIH2O, cast and made insoluble with methanol) to bind ﬁbrinogen as a mechanism by which the alternative complement pathway is activated in vivo. However, compared to two reference materials, polystyrene and poly(2-hydroxyethyl methacrylate), ﬁbroin ﬁlms bound ﬁbrinogen to a lesser extent . C3 and IgG, components of the human plasma complement system bound similarly when the silk was compared to the reference materials. The authors concluded that C3 binding may be the result of speciﬁc binding to hydrophobic patches (e.g., bsheets) of ﬁbroin. When compared to the reference materials after 24 h in vitro, diminished interleukin-1b
Rat/abdominal wall muscle
Rabbit/cornea, sclera and ocular muscle
Rabbit/abdominal wall muscle
Unknown/assumed black braided
Unknown/assumed virgin silk
Type of silk: virgin=raw silk containing sericin; black braided=extracted silk ﬁbroin ﬁbers (e.g., no sericin) coated in waxes or silicone; ﬁbroin ﬁlm=extracted and solubilized ﬁbroin cast and insolubilized with methanol.
Rat/subcutaneous Black braided
Foreign body response (proteolytic degradation)
Rat/subcutaneous Unknown/assumed black braided
Salthouse et al. 
Lam et al. 
In vitro Extracted ﬁbroin ﬁlm
Unknown/assumed foreign body response Unknown/assumed foreign body response Foreign body response (proteolytic degradation) Foreign body response (proteolytic degradation)
Bucknall et al. 
Minoura et al. 
B10% weight loss 5 days following enzymatic digestion 55% loss in tensile strength 6 weeks in vivo 83% loss in tensile strength 10 weeks in vivo Fragmentation at 6 weeks; not detected at 24 weeks Reduced number of ﬁlaments and diameter at 42 days; absorption at 90 days in vivo 80% decrease in tensile strength at 12 weeks; 0% strength at 2 years; decrease in the number of ﬁbers observed histologically; fragmentation following 4 weeks in vivo
In vivo/in vitro Type of silka
Table 5 Evidence of silk degradation in vitro and in vivo
According to the US Pharmacopeia an absorbable (suture) biomaterial is deﬁned as one that ‘loses most of its tensile strength within 60 days’ post-implantation in vivo. Within this deﬁnition, silk is correctly classiﬁed as non-degradable. However, according to the literature, silk is degradable but over longer time periods due to proteolytic degradation usually mediated by a foreign body response [31,34,41,52]. Several studies detail variable rates of silk absorption in vivo dependent on the animal model and tissue implantation site (Table 5). In general, silk ﬁbers lose the majority of their tensile strength within 1 year in vivo, and fail to be recognized at the site within 2 years . Silk studies in vitro have demonstrated that proteases such as chymotrypsin will cleave the less-crystalline regions of the protein to peptides which are then capable of being phagocytosed for further metabolism by the cell. Furthermore, protease cocktails  and chymotrypsin (known to be produced by macrophages) are capable of enzymatically degrading silk . Of interest, the silkworm B. mori produces a protease inhibitor in the silk gland embedding it within the silk cocoon for protection against premature proteolytic degradation . In a comparative study of six absorbable and four non-degradable sutures implanted circumferentially under the skin of rats, silk lost 55% of its tensile
5. Silk degradation
production from mononuclear cells isolated from human plasma incubated with ﬁbroin was observed . Uff et al.  examined the effects of soluble factors from sutures on macrophage activation (e.g., attachment, phagacytosis and the production of lysozyme and proinﬂammatory tumor necrosis factor (TNF)) in vitro. Soluble factors were acquired by subjecting sterile sutures to ultrasound for 1 h in detergent. Soluble factors from silk were found to elicit the highest phagocytic response from macrophages when compared to catgut, PDSTM, steel, nylon and VicrylTM. However, VicrylTM induced the highest response when characterizing macrophage adherence and TNF production. PDSTM induced the highest production of lysozyme of the group of sutures extracted. The authors failed to characterize the soluble factors produced by soniﬁcation of the suture materials. In the case of silk, the resulting response from macrophages could be due to a variety of factors including residual sericin, waxes or silicones used in manufacture of the sutures, or the speciﬁc size of ﬁbroin particles or crystals potentially generated. Thus, the response may be completely independent of actual silk ﬁbroin material properties and rather a function of the coating and/or geometry and size of particles produced.
Greenwald et al. 
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
Degree and measure of degradation
E8 E8 E8 E8 E7 E8 E8 E8 E8 E8
a Strength of initial suture prior to implantation (0 weeks) and at 6 weeks following in vivo circumferential subcutaneous implantation in a rat model. Fragmented sutures that were unable to be harvested following implantation at 6 weeks were assumed to have lost 100% of their tensile integrity. b Elastic modulus of sutures (N/m2) prior to implantation and following 6 weeks in vivo. c Type of silk (e.g., virgin or black braided) was not described. It is assumed to be black-braided silk.
100 100 100 100 85.8 26TM 16.1 0 0 6.9 3.00 2.62 1.41 1.56 9.87 1.00 2.42 1.04 1.00 2.47 B100 B100 B100 B100 86.5 86.1 55.2 44.4 25.6 6.8 Fragmented Fragmented Fragmented Fragmented 9.72 E13 8.29 E13 3.80 E13 2.54 E14 2.99 E14 2.32 E14 E14 E14 E14 E14 E14 E14 E13 E14 E14 E14 1.42 3.46 2.30 2.28 7.20 5.96 8.48 4.57 4.02 2.49 (polyglactin 910) Vicryl DexonTM (polyglycolic acid) CatgutTM (collagen) Chromic CatgutTM (cross-linked collagen) PDSTM (polydioxanone) MaxonTM(polyglyconate) Silkc EthilonTM (nylon) ProleneTM (polypropylene) EthibondTM (polyester)
— — — — 7.13 E7 7.4 E7 2.03 E8 1.07 E8 1.01 E8 2.30 E8
0 Weeks % Decrease 0 Weeks
Tangent elastic modulus (N/m2)b Strength (N/m2)a Suture name
Table 6 Material properties of 10 common sutures following 6 weeks of subcutaneous implantation in a rat model. Values at time 0–6 weeks taken from Table 1 of Ref. 
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
Table 7 Percent loss in suture mechanical tensile strength over time subcutaneously implanted in a rat model. Durability data was taken from Table 3 of Ref.  Suture
Polyglycolic acid Silk, black braided Multiﬁlament nylon Monoﬁlament nylon
Time post-implantation 10 days
65% 29% 16% 3%
92% 73% 19% 7%
99% 83% 22% 16%
strength and 16% of its elastic modulus 6 weeks postimplantation  (Table 6). In a rat model with subcutaneous implantation, silk ﬁbers lost 29% of their tensile strength at 10 days, 73% at 30 days and 83% 70 days post-implantation (Table 7) . In abdominal wound closures in the rat, silk promoted a moderate foreign body response compared to mono- and multiﬁlament nylon and polyglycolic acid (PGA) sutures . However, common to all sutures, inﬂammation was required as the main mechanism for degradation. Lam et al.  described silk as biodegradable due to its susceptibility to proteolytic enzymes. The study compared dry-spun hot-drawn poly(l-lactic acid) (PLLA) ﬁbers to several absorbable and non-degradable sutures in the muscle layer surrounding the abdomen of rats. PLLA, PDSTM, VicrylTM, and black braided silk showed signs of degradation after 2 weeks in vivo as determined by scanning electron microscopy. All sutures, in addition to monoﬁlament nylon, provoked a chronic inﬂammatory response at 2 weeks. At 6 and 12 weeks in vivo, the authors were unable to retrieve silk due to fragmentation. At 24 weeks, neither silk nor inﬂammation was observed in vivo most likely due the rapid degradation of silk by proteolytic enzymatic digestion. Inﬂammation subsided by 6 weeks in vivo for Vicryl; a chronic inﬂammatory response was present surrounding PLLA at 80 weeks in vivo, the ﬁnal time point of the study. In general, silk is slowly absorbed in vivo. The rate of absorption is dependent upon the implantation site, mechanical environment, and variables related to the health and physiological status of the patient, the type (virgin silk versus extracted black braided ﬁbroin), and the diameter of the silk ﬁber [31,34,52]. Furthermore, alterations in silk processing may cause conformational changes in the protein structure potentially increasing or decreasing susceptibility to degradation. None of these variables has been studied in detail; therefore, it is difﬁcult to gain a clear understanding of the relationships between structure, processing and degradability. Regardless, silk protein ﬁbers will degrade in vivo; rates are variable depending on the factors listed above.
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
It should be recognized that amyloid-like deposits in Alzheimer’s and related diseases are often associated with b-sheet structures, particularly cross-beta crystals . Similar structures are also implicated in membraneassociated cytotoxicity . It is unknown if silks, such as those from silkworm, spiders or genetic variants thereof, will negatively inﬂuence biological function in a similar mode as these amyloid systems. This issue should be addressed over time as tissue-engineering studies move forward. The outcomes of these studies would inﬂuence the types of tissue applications that should be addressed with silk. It is encouraging that no amyloidrelated problems have been reported throughout the literature to date associated with silk ﬁbers, despite their extensive use in the clinical setting for many centuries. As the use of silk-based biomaterials broadens, presumably the ASTM would be involved to establish standard guidelines for this type of assessment.
6. Scaffolds for tissue engineering The emergence of tissue engineering has increased the demand for a diverse portfolio of biomaterials to support the development of tissues in vitro prior to implantation in vivo. The biomaterial or matrix plays a key role in communicating or transducing environmental cues to cells seeded within or on the matrix. In essence, the matrix acts as the translator between the local (e.g., mechanical) environment (either in vitro or in vivo) and the developing tissue, aiding in the development of biologically viable functional tissue. The matrix must support cell attachment, spreading, growth and differentiation. In most instances it is advantageous if the matrix degrades into biocompatible fragments or monomers capable of being metabolized by host cells; however, the rate of degradation must match or be less than the rate of tissue ingrowth and development. This
balance assures appropriate mechanical and physiological compatibility during integration of the host and/or implanted tissue in vivo. A mismatch in these rates can lead to premature failure of the tissue. Silk ﬁbroin offers versatility in matrix scaffold design for a number of tissue engineering needs (Table 8) in which mechanical performance and biological interactions are major factors for success, including bone, ligaments, tendons, blood vessels and cartilage. Silk ﬁbroin can be processed into foams, ﬁlms, ﬁbers and meshes. Inouye et al.  demonstrated the utility of a silk ﬁbroin ﬁlm in culturing animal cells (SE1116, human colon adenocarcinoma; KB, human mouth epidermoid carcinoma; Colo201, human colon adenocarcinoma; QG56, human lung carcinoma) in comparison to a collagen matrix. Films of both ﬁbroin and collagen supported equivalent cell growth after 5 days in cell culture conditions. Minoura et al.  compared the ability of ﬁbroin and sericin ﬁlms, as well as a control, collagen (cast bovine acid soluble) ﬁlm, in supporting attachment, spreading and growth of the L-929 ﬁbroblast cell line. The results indicated that ﬁbroin and collagen ﬁlms were equivalent in their ability to support cell attachment, physiological morphology and growth when compared to the sericin ﬁlm. These results support the concept that extracted ﬁbroin free of sericin is a suitable matrix for cell and tissue culture. In our own studies, ﬁbroin ﬁlms induced bone tissue growth in vitro when seeded with osteoblasts . When the ﬁlms were chemically decorated with the peptide RGD to promote integrin interactions for adhesion, the induction of bone formation in vitro was signiﬁcantly enhanced. The response was determined based on increased alkaline phosphatase levels, upregulation of bone-speciﬁc transcripts, and calciﬁcation levels over 4 weeks. Similar responses were not observed when parathyroid hormone was immobilized and also assayed with osteoblasts. The utility of a protein matrix offering
Table 8 Examples of silk’s utility as a matrix material in tissue engineering Silk form
Supported cell type in vitro
L-929 mouse ﬁbroblast
Comparable growth rates to collagen ﬁlms
Minoura et al. 
SE1116 (human colon adenocarcinoma); KB (human mouth epidermoid carcinoma); Colo201 (human colon adenocarcinoma); QG56 (human lung carcinoma)
Comparable growth rates to collagen ﬁlms as well as rates of protein production of carcinoembryonic antigen (CEA)
Inouye et al. 
Saos-2 (human osteoblast-like cells)
Bone formation was evident on ﬁbroin ﬁlms, but was enhanced on RGD-coupled matrices
Soﬁa et al. 
hBMSC (human bone marrow stromal cells)
Supports bone nodule formation from adult stem cells
hBMSC; human adult anterior cruciate ligament ﬁbroblasts
Supports ligament speciﬁc development in vitro
Altman et al. 
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
a diversity of sites (e.g., amino acids) for selective chemical couplings for tissue engineering is a beneﬁt of the silk system. Bone tissue formation was a logical target tissue for silk due to the unique mechanical properties of the protein in ﬁber and ﬁlm forms. Recent research with silk has focused on the development of a wire rope matrix for the development of autologous tissue engineered anterior cruciate ligaments (ACL) using a patient’s own adult stem cells . Biologically compatible and mechanically robust biomaterials are critical based on the stringent requirements of ligaments and the dynamic and demanding mechanical environment of the knee. Human bone marrow stromal cells (BMSCs) cultured in collagen gels were grown in a mechanically dynamic environment relevant to that present in vivo leading to the formation of ligament ﬁbroblasts (from the BMSCs) and mature tissue development in vitro . However, the poor integrity of the collagen gels and the demanding and dynamic intra-articular mechanical and biochemical environment of the knee have prompted renewed interest in silk as a long term absorbable material with good mechanical integrity and biocompatibility.
Collagen ﬁbers have been used as a matrix biomaterial to support de novo ligament formation in vivo with limited success. In the early 1990s Dunn et al.  reported initial work on the development of a ligament prosthesis involving a collagenous ACL prosthesis . Results showed inconsistent neoligament formation and signiﬁcant weakening of the prosthesis in a rabbit model. Enhanced scaffolds were examined including a collagen ﬁber-PLA composite to further maintain mechanical integrity allowing for neoligament tissue ingrowth . In both studies, only half of the structures remained intact 4 weeks post-reconstruction suggesting that this composition (collagen and PLA) was inadequate for the rigorous in vivo environment of the ACL. Silk’s unique mechanical properties, coupled with the ability to weave the ﬁbers into a wire-rope geometry provides control over the matrix’s ﬁnal mechanical properties (i.e., matrix stiffness can be altered by adjusting the pitch angle of a wire rope) to mimic the mechanical properties of the native ACL and support host tissue ingrowth offering new options in ACL tissue engineering. Pilot scale manufacturing equipment has been developed for the fabrication of ACL wire-rope
Fig. 1. (A) Pilot-scale manufacturing equipment for the fabrication of silk wire-rope matrices showing (i) two computer controlled twisting machines, (ii) a 160 l stainless steel water bath with immersion heaters, and (iii) a custom designed ﬁber extraction rack holding 94 individual groups of ﬁbers to be extracted free of sericin; (B) a close up of the extraction rack containing 94 individually anchored groups of ﬁbers; (C) spring-loaded clamps used to keep ﬁbers or groups of ﬁbers in equal tension during extraction, rinsing and drying.
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
ﬁbroin matrices (Fig. 1). A 160 l stainless steel water bath (Fig. 1A) and custom designed ﬁber extraction racks to keep individual ﬁbers or groups of ﬁbers in equal tension were developed. The extraction rack was designed to anchor up to 94 individual ﬁbers or groups of ﬁbers (Fig. 1B) with spring-loaded clamps (Fig. 1C). The water bath (214 cm 61 cm 15 cm) combined with two immersion heaters and an external pump allow recirculating ﬂow of the extraction broth at 901C over the rack containing the silk. Following sericin extraction, two computer controlled twisting machines (Figs. 1A and 2) were developed to fabricate wire-rope matrices with desired geometries (e.g., material properties). One of many fabricated matrices is shown in Fig. 3. Conﬁrming silks utility as a biocompatible material for in vitro ligament tissue engineering, BMSCs were shown to attach, spread and proliferate on the silk ﬁber matrices . Scanning electron microscopy (SEM) images of virgin silk and extracted silk (Fig. 4) as well as BMSC seeded ﬁbroin wire-rope matrices are shown (Fig. 5). BMSC are able to attach within 5 min (Fig. 5A), initially spread at 1 h (Fig. 5B), and form conﬂuent cell sheets with possible extracellular matrix formation 7 days and 14 days post-seeding (Figs. 5C and D). It is generally accepted in the literature that silk will slowly degrade in vivo as a function of proteolytic attack. However, in vitro in immune system deﬁcient tissue culture conditions, sericin-extracted ﬁbroin silk ﬁbers retained their initial tensile integrity over 21 days
. In vitro studies of the extracted silk ﬁbroin exhibited a negligible response from macrophages as assessed by cytokine release in vitro (unpublished data). As a result, appropriate, directed and rigorous mechanical stimuli can be communicated to adhered stem cells in vitro without concern for premature graft mechanical failure; however, the effects of mechanical fatigue on graft integrity will need to be characterized for each culture condition and variant matrix geometry. We have shown that the application of mechanical stimuli will induce BMSC ligament speciﬁc differentiation and matrix formation in vitro . The utility of this tissue engineering approach in combination with a mechanical robust silk matrix is the potential inhibition of a FBR following implantation in vivo due to the
Fig. 3. One of many silk cords manufactured by the twisting equipment. The silk cord shown contains 5 levels of twisting hierarchy and 540 individual ﬁbers twisted to approximate the stiffness of the human ACL.
Fig. 2. A close-up view of the twisting machines showing the motor controlled spring-loaded clamps. The clamps can anchor from 2 to 6 ﬁbers or groups of ﬁbers for twisting.
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
Fig. 4. (A) SEM of raw virgin B. mori silk ﬁbers prior to extraction showing the gum-like sericin proteins coating the core ﬁbroin and (B) following extraction at 901C for 60 min in conditions previously described  showing the individual smooth ﬁbroin ﬁlaments following the removal of the covering sericin.
Fig. 5. (A) Initially attached BMSCs on the ﬁbroin cord shown in Fig. 3, 5 min following seeding of the ﬁbers with 2 million cells/ml (1 ml total per 3 cm of silk cord). (B) Initial cell spreading on the ﬁbroin 1 h after seeding. (C) Seven days post-seeding with a cell and ECM sheet evident. (D) Fourteen days following seeding, thick encapsulation of the matrix by cells and ECM.
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
presentation of autologous ligament tissue (derived from the BMSC) to the host. This approach should allow both inﬁltration of host tissue and the in vitro developed ligament tissue incorporated into and surrounding the matrix to form mature functional, biologically viable autologous ligament tissue. Studies are currently ongoing to identify an optimal matrix geometry and stiffness to best support tissue ingrowth both in vitro and in vivo. Furthermore, silk’s high ultimate tensile stress (N/mm2) provides signiﬁcant void volume in vivo occupying only B12% of the space of a human ACL (given a human ACL 27 mm in length and 8 mm in diameter). We suspect, following angiogenesis and revascularization of the tissue engineered ligament within 8–12 weeks in vivo, the core original silk matrix will be proteolytically degraded and metabolized in vivo. The effects of the rigorous mechanical knee joint environment on matrix fatigue life over the long term remain to be determined but will clearly guarantee the eventual failure of the silk matrix in vivo, a desired goal to ensure biologically viable, host ligamentous tissue eventually sustains the functional roles of the ACL over the life of the patient. In terms of matrices for tissue engineering, the novel mechanical properties of silk in ﬁlm, ﬁber (Table 1) or sponge forms, coupled with the facile chemical decoration, the potential to form complex rope designs to match functional requirements for speciﬁc tissues, and the slow rate of degradation in vivo to provide adequate robust support, suggest that silks offer many beneﬁts when compared to other types of natural or synthetic degradable ﬁbers, ﬁlms and foams. For example, in the case of bone, biomaterials that can provide robust support during compression would be advantageous, and silks are known to function well under compression with little evidence for cracking or crazing under conditions in which synthetic high performance ﬁbers fail . Furthermore, in the case of ligaments, the high tensile strength of silks provides a strong advantage in matching ligament function to immediately restore knee function, a feature difﬁcult to achieve with collagen . Silks ﬁbers and ﬁlms are often prepared from resolubilized protein after dissolution in high concentrations of lithium salts or calcium nitrate. Once soluble, the proteins can be dialyzed, lyophilized and resolubilized in organic solvents such as hexaﬂuoroisopropanol or in water for limited periods of time depending on concentration. In the case of ﬁber formation, silks [65,66] and collagens  have been electrospun to form nanometer-scale diameter ﬁbers. Thus, modulation in ﬁber diameters from the native 10’s of microns in the case of B. mori to submicron by electrospinning offers a range of morphologies for cell interactions. It is also interesting to note that unrestrained dragline silk from N. clavipes will supercontract. However, when embedded in a material or restrained, this unusual feature
is lost. Silkworm silk ﬁbers from B. mori do not supercontract.
7. Conclusions B. mori silk ﬁbers are composed primarily of two types of proteins: (1) sericin, the antigenic gum-like protein surrounding the ﬁbers and (2) ﬁbroin, the core ﬁlaments of silk comprised of highly organized b-sheet crystal regions and semi-crystalline regions responsible for silk’s elasticity compared to ﬁbers of similar tensile integrity. Silk has been used in biomedical applications for centuries primarily for the ligation of wounds. Virgin silk suture (containing sericin) induces hypersensitivity in patients, causing a Type I allergic reaction. Exposure to silk debris (e.g., broken virgin silk ﬁbers used in bedding and fabrics) may sensitize patients to silk causing adverse allergic reactions when silk is used as a suture material. Sericin, identiﬁed as the antigenic agent of silk, is removed and replaced with a wax or silicone coating in commercial black braided silk sutures. As a result, T-cell mediated hypersensitivity has not been observed in response to black braided silk in the literature. Unfortunately, poor documentation of the exact type of silk suture used when describing host responses to silk in the literature has led to confusion regarding the utility of silk in biomedical applications. As a result, the use of silk over the past 20 years has declined since the arrival of commonly used absorbable and non-degradable synthetics such as VicrylTM and EthibondTM. Another misconception about silk revolves around its ability to degrade in vivo. Deﬁned as non-degradable by the USP because it retains the majority of its tensile strength beyond 60 days in vivo, silk is commonly thought of as a permanent suture once implanted into the body. As a protein, silk is susceptible to proteolytic degradation, but over a longer time periods. Based on the literature, it is apparent that silk ﬁbroin will lose the majority of its tensile strength within 1 year in vivo. In some cases, the silk or the features associated with inﬂammation cannot be found at the implantation site within months following surgery. Therefore, silk is a long-term absorbable suture. Silk ﬁbroin elicits a foreign body response following implantation in vivo. Yet the response is comparable to the most popular synthetic materials in use today as biomaterials, and is dependent upon the implantation site and model used for investigation. In rare cases a granuloma may form as a result of an abandoned phagocytic response to silk by macrophages and giant body cells. Again, the response is dependent on the implantation site of the silk. It is known that within blood, silk is highly thrombic. Clearly, this results from a unique feature of the silk ﬁbroin protein to bind
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
components of the clotting cascade such as ﬁbrin and ﬁbrinogen. However, in most cases, the response is moderate and subsides with time. To examine the material properties of silk ﬁbroin in relation to other common degradable and non-degradable biomaterials in vivo, comparisons should be made by equating surface area of the materials under investigation. Individual silk ﬁbroin ﬁlaments, due to their small diameter (B5 mm) increase the surface area to volume ratio of silk sutures when compared to other biomaterials where the equating factor is typically ﬁnal suture diameter. As a result, in cases that demonstrate a greater foreign body response to silk in vivo, the comparison may not be equitable to the inherent material properties of silk ﬁbroin. Therefore, silk ﬁbroin when utilized as ﬁlms, foams and ﬁbers, may offer a ‘new’ alternative biomaterial for use as matrices in tissue engineering where mechanically robust, long-term degradable materials are needed.
Acknowledgements We thank the NIH (R01 DE13405-01 and R01 AR46563-01), the NSF (DMR-0090384) and Tissue Regeneration, Inc., for support of this research.
References  Kaplan DL, Mello SM, Arcidiacono S, Fossey S, Senecal K, Muller W. Silk. In: McGrath K, Kaplan DL, editors. Protein based materials. Boston: Birkhauser, 1998. p. 103–31.  Kaplan DL, Adams WW, Farmer B, Viney C. Silk: biology, structure, properties and genetics. In: Kaplan DL, Adams WW, Farmer B, Viney C, editors. Silk polymers: materials science and biotechnology. ACS Symp Ser 1994;544:2–16.  Kaplan DL, Fossey S, Viney C, Muller W. Self-organization (assembly) in biosynthesis of silk ﬁbers—a hierarchical problem. In: Aksay IA, Baer E, Sarikaya M, Tirrell DA, editors. Hierarchically structured materials. Materials Res Symp Proc 1992;255:19–29.  Guerette PA, Ginzinger DG, Weber BHF, Gosline JM. Silk properties determined by gland-speciﬁc expression of a spider ﬁbroin gene family. Science 1996;272:112–5.  Cappello J. The biological production of protein polymers and their use. Trends Biotechnol 1990;8:309–11.  Xu M, Lewis RV. Structure of a protein superﬁber: spider dragline silk. Proc Natl Acad Sci USA 1990;87:7120–4.  Gosline JM, Denny MW, DeMont ME. Spider silk as rubber. Nature 1984;309:551–2.  Hayashi CY, Lewis RV. Molecular architecture and evolution of a modular spider silk protein gene. Science 2000;287:1477–9.  Arcidiacono S, Mello C, Kaplan DL, Cheley S, Bayley H. Puriﬁcation and characterization of recombinant spider silk expressed in Escherichia coli. Appl Microbiol Biotechnol 1998;49:31–8.  Hayashi CY, Lewis RV. Evidence from ﬂagelliform silk cDNA for the structural basis of elasticity and modular nature of spider silks. J Mol Biol 1998;275:773–84.
 Hinman MB, Lewis RV. Isolation of a clone encoding a second dragline silk ﬁbroin. J Biol Chem 1992;267:19320–4.  Zhou CZ, Confalonieri F, Medina N, Zivanovic Y, Esnault C, Yang T, Jacquet M, Janin J, Duguet M, Perasso R, Li ZG. Fine organization of Bombyx mori ﬁbroin heavy chain gene. Nucleic Acids Res 2000;28:2413–9.  Cunniff PM, Fossey SA, Auerbach MA, Song JW, Kaplan DL, Adams WW, Eby RK, Mahoney D, Vezie DL. Mechanical and thermal properties of dragline silk from the spider, Nephila clavipes. Polym Adv Technol 1994;5:401–10.  Gosline JM, DeMont ME, Denny MW. The structure and properties of spider silk. Endeavour 1986;10:37–43.  Lazaris A, Arcidiacono S, Huang Y, Zhou JF, Duguay F, Chretien N, Welsh EA, Soares JW, Karatzas CN. Spider silk ﬁbers spun from soluble recombinant silk produced in mammalian cells. Science 2002;295:472–6.  Hood EE, Jilka JM. Plant-based production of xenogenic proteins. Curr Opin Biotechnol 2000;10:382–6.  Wilson D, Valluzzi R, Kaplan DL. Conformational transitions in model silk peptides. Biophys J 2000;78:2690–701.  Szela S, Avtges P, Valluzzi R, Winkler S, Wilson D, Kirschner D, Kaplan DL. Reduction-oxidation control of b-sheet assembly in genetically engineered silk. Biomacromolecules 2000;1: 534–42.  Winkler S, Wilson D, Kaplan DL. Controlling b-sheet assembly in genetically engineered silk by enzymatic phosphorylation/ dephosphorylation. Biochemistry 2000;39:12739–46.  Valluzzi R, Szela S, Avtges P, Kirschner D, Kaplan DL. Methionine redox controlled crystallization of biosynthetic silk spidroin. J Phys Chem B 1999;103:11382–92.  Winkler S, Szela S, Avtges P, Valluzzi R, Kirschner DA, Kaplan DL. Designing recombinant spider silk proteins to control assembly. Int J Biol Macro 1999;24:265–70.  Winkler S, Kaplan DL. Molecular biology of spider silk. Rev Mol Biotech 2000;74:85–93.  Heslot H. Artiﬁcial ﬁbrous proteins: a review. Biochimie 1998;80:19–31.  Kadler KE. Fibril forming collagens. In: Sheterline P, editor. Protein proﬁles: extracellular matrix, vol. 1. London, UK: Academic Press, 1995.  Moy RL, Lee A, Zalka A. Commonly used suture materials in skin surgery. Am Fam Physician 1991;44:2123–8.  Minoura N, Aiba S, Gotoh Y, Tsukada M, Imai Y. Attachment and growth of cultured ﬁbroblast cells on silk protein matrices. J Biomed Mater Res 1995;29:1215–21.  Moynihan BGA. The ritual of a surgical operation. Br J Surg 1920;8:27–35.  Hollander DH. Interstitial cystitis and silk allergy. Med Hypotheses 1994;43:155–6.  Wen CM, Ye ST, Zhou LX, Yu Y. Silk-induced asthma in children: a report of 64 cases. Ann Allergy 1990;65:375–8.  Kurosaki S, Otsuka H, Kunitomo M, Koyama M, Pawankar R, Matumoto K. Fibroin allergy: IgE mediated hypersensitivity to silk suture materials. Nippon Ika Daigaku Zasshi 1999;66: 41–4.  Rossitch Jr. E, Bullard DE, Oakes WJ. Delayed foreign-body reaction to silk sutures in pediatric neurosurgical patients. Childs Nerv Syst 1987;3:375–8.  Dewair M, Baur X, Ziegler K. Use of immunoblot technique for detection of human IgE and IgG antibodies to individual silk proteins. J Allergy Clin Immunol 1985;76:537–42.  Zaoming W, Codina R, Fernandez-Caldas E, Lockey RF. Partial characterization of the silk allergens in mulberry silk extract. J Inv Allergy Clin Immunol 1996;6:237–41.  Soong HK, Kenyon KR. Adverse reactions to virgin silk sutures in cataract surgery. Ophthalmology 1984;91:479–83.
G.H. Altman et al. / Biomaterials 24 (2003) 401–416
 Postlethwait RW. Long-term comparative study of nonabsorbable sutures. Ann Surg 1970;171:892–8.  Postlethwait RW. Tissue reaction to surgical sutures. In: Dumphy JE, Van Winkle W, editors. Repair and regeneration. New York: McGraw-Hill, 1969. p. 263–85.  Postlethwait RW, Dillon MD, Reeves JW. Experimental study of silk suture. Arch Surg 1962;84:698–702.  Morrow FA, Kogan SJ, Freed SZ, Laufman H. In vivo comparison of polyglycolic acid, chromic catgut and silk in tissue of the genitourinary tract: an experimental study of tissue retrieval and calculogenesis. J Urol 1974;112:655–8.  Nebel L, Rosenberg G, Tobias B, Nathan H. Autograft suture in peripheral nerves. Eur Surg Res 1977;9:224–34.  Peleg H, Rao UN, Emrich LJ. An experimental comparison of suture materials for tracheal and bronchial anastomoses. J Thorac Cardiovasc Surg 1986;34:384–8.  Lam KH, Nijenhuis AJ, Bartels H, Postema AR, Jonkman MF, Pennings AJ, Nieuwenhuis P. Reinforced poly(l-Lactic Acid) ﬁbers as suture material. J Appl Biomater 1995;6:191–7.  Anderson JM. Inﬂammation, wound healing, and the foreign body response. In: Ratner BD, Hoffman AS, Schoen FJ, Lemons JE, editors. Biomaterials science: an introduction to materials in medicine. Boston: Academic Press, 1996. p. 165–72.  Foschi D, Corsi F, Cellerino P, Rizzi A, Morandi E, Trabucchi E. Angiogenic effects of suture biomaterials. An experimental study in rats. Eur Surg Res 2001;33:16–20.  Setzen G, Williams EF. Tissue response to suture materials implanted subcutaneously in a rabbit model. Plast Reconstr Surg 1997;100:1788–95.  Bucknall TE, Teare L, Ellis H. The choice of a suture to close abdominal incisions. Eur Surg Res 1983;15:59–66.  Wong PC, Crain EJ, Nguan O, Watson CA, Racanelli A. Antithrombotic actions of selective inhibitors of blood coagulation factor Xa in rat models of thrombosis. Thromb Res 1996;83:117–26.  Dahlke H, Dociu N, Thurau K. Thrombogenicity of different suture materials as revealed by scanning electron microscopy. J Biomed Mater Res 1980;14:251–68.  Lee KY, Kong SJ, Park WH, Ha WS, Kwon IC. Effect of surface properties on the antithrombogenicity of silk ﬁbroin/S-carboxymethyl kerateine blend ﬁlms. J Biomater Sci Polym Ed 1998;9:905–14.  Sakabe H, Ito H, Miyamoto T, Noishiki Y, Ha WS. In vivo blood compatibility of regenerated silk ﬁbroin. Sen-I Gakkaishi 1989;45:487–90.  Santin M, Motta A, Freddi G, Cannas M. In vitro evaluation of the inﬂammatory potential of the silk ﬁbroin. J Biomed Mater Res 1999;46:382–9.  Uff CR, Scott AD, Pockley AG, Phillips RK. Inﬂuence of soluble suture factors on in vitro macrophage function. Biomaterials 1995;16:355–60.  Salthouse TN, Matlaga BF, Wykoff MH. Comparative tissue response to six suture materials in rabbit cornea, sclera, and ocular muscle. Am J Ophthalmol 1977;84:224–33.  Ethicon, Inc., Wound closure manual. The suture: speciﬁc suturing materials. Non-absorbable sutures. Somerville, NJ: Ethicon, Inc. [copyright 2000, Chapter 2].
 Minoura N, Tsukada M, Nagura M. Physico-chemical properties of silk ﬁbroin membrane as a biomaterial. Biomaterials 1990;11:430–4.  Asakura T, Demura M, Date T, Miyashita N, Ogawa K, Williamson MP. NMR study of silk I structure of Bombyx mori silk ﬁbroin with N-15- and C-13-NMR chemical shift contour plots. Biopolymers 1997;41:193–203.  Kurioka A, Yamazaki M, Hirano H. Primary structure and possible functions of a trypsin inhibitor of Bombyx mori. Eur J Biochem 1999;259:120–6.  Greenwald D, Shumway S, Albear P, Gottlieb L. Mechanical comparison of 10 suture materials before and after in vivo incubation. J Surg Res 1994;56:372–7.  Kourie JI, Shorthouse AA. Properties of cytotoxic peptideformed ion channels. Am J Physiol Cell Physiol 2000;278: C1063–87.  Inouye K, Kurokawa M, Nishikawa S, Tsukada M. Use of Bombyx mori silk ﬁbroin as a substratum for cultivation of animal cells. J Biochem Biophys Meth 1998;37:159–64.  Soﬁa S, McCarthy MB, Gronowicz G, Kaplan DL. Functionalized silk-based biomaterials for bone formation. J Biomed Mater Res 2001;54:139–48.  Altman GH, Horan RL, Lu H, Moreau J, Martin I, Richmond JC, Kaplan DL. Silk matrix for tissue engineered anterior cruciate ligaments. Biomaterials 2002;23:4131–41.  Altman GH, Horan RL, Martin I, Farhadi J, Stark PRH, Volloch V, Richmond JC, Vunjak-Novakovic, Kaplan DL. Cell differentiation by mechanical stress. FASEB J 2001;16:270–2 (print) and 10:1096 (electronic).  Dunn MG, Tria AJ, Kato P, Bechler JR, Ochner RS, Zawadski JP, Silver FH. Anterior cruciate ligament reconstruction using a composite collagenous prosthesis. Am J Sports Med 1992;20: 507–15.  Dunn MG, Bellincampi LD, Tria AJ, Zawadski JP. Preliminary development of a collagen-PLA composite for ACL reconstruction. J Appl Polym Sci 1997;63:1423–8.  Zarkoob S, Reneker DH, Eby RK, Hudson SD, Ertley D, Adams WW. Generation of synthetic elastin-mimetic small diameter ﬁbers and ﬁber networks. Polym Preprints Am Chem Soc 1998;39:244–5.  Jin H-J, Fridrikh SV, Rutledge GC, Kaplan DL. Electrospinning Bombyx mori silk with poly(ethylene oxide). Biomacromolecules, in press.  Matthews JA, Wnek GE, Simpson DG, Bowlin GL. Electrospinning of collagen nanoﬁbers. Biomacromolecules 2002;3:232–8.  Perez-Rigueiro J, Viney C, Llorca J, Elices M. Mechanical properties of single-brin silkworm silk. J Appl Polym Sci 2000;75:1270–7.  Pins GD, Christiansen DL, Patel R, Silver FH. Self-assembly of collagen ﬁbers: inﬂuence of ﬁbrillar alignment and decorin on mechanical properties. Biophys J 1997;73:2164–72.  Engelberg I, Kohn J. Physicomechanical properties of degradable polymers used in medical applications: a comparative study. Biomaterials 1991;12:292–304.  Gosline JM, Guerette PA, Ortlepp CS, Savage KN. The mechanical design of spider silks: from ﬁbroin sequence to mechanical function. J Exp Biol 1999;202(Pt 23):3295–303.